Presentation on theme: "ECDP332 Concrete Technology Faculty of Applied Engineering and Urban Planning Civil Engineering Department Lect. 2 2 nd Semester 2008/2009 UP Copyrights."— Presentation transcript:
ECDP332 Concrete Technology Faculty of Applied Engineering and Urban Planning Civil Engineering Department Lect. 2 2 nd Semester 2008/2009 UP Copyrights 2009 Concrete Technology Eng: Eyad Haddad
Chapter 2: Portland Cement Cement is a pulverized material that develops binding forces due to a reaction with water. Hydraulic Cement → Stable under water Nonhydraulic Cement → Products of hydration are not resistant to water (i.e. limestone) Hydraulic cements Cements that harden by reaction with water and form a water- resistant product.
Portland Cement (P.C.) Portland cement is a hydraulic cement capable of setting, hardening and remains stable under water. It is composed of calcium silicates and some amount of gypsum. P.C components: Clay(sio2+Al2o3+Fe2o3) + calcium silicates (caco3) + Natural Sand + gypsoum(caso4+2H2o)
Modified P. Cement (1- Blended P. Cements) Blended cement, as defined in ASTM C 595, is a mixture of portland cement and blast furnace slag (BFS) or a "mixture of portland cement and a pozzolan (most commonly fly ash)." The use of blended cements in concrete reduces mixing water and bleeding, improves finishability and workability, enhances sulfate resistance, inhibits the alkali-aggregate reaction, and lessens heat evolution during hydration, thus moderating the chances for thermal cracking on cooling.
Modified Portland Cement (2- Expansive Cement) Expansive cement, as well as expansive components, is a cement containing hydraulic calcium silicates (such as those characteristic of portland cement) that, upon being mixed with water, forms a paste, that during the early hydrating period occurring after setting, increases in volume significantly more than does portland cement paste. Expansive cement is used to compensate for volume decrease due to shrinkage and to induce tensile stress in reinforcement. Expansive cement concrete used to minimize cracking caused by drying shrinkage in concrete slabs, pavements, and structures is termed shrinkage-compensating concrete.
Modified Portland Cement (2- Expansive Cement) Cont. Self-stressing concrete is another expansive cement concrete in which the expansion, if restrained, will induce a compressive stress high enough to result in a significant residual compression in the concrete after drying shrinkage has occurred.
Manufacturing of Portland Cement Calcium silicates are the primary constituents of portland cement. Raw material for P.C. is Calcium & Silica Calcium: Limestone, chalk, etc (CaO+CO2) Silica: Clays and shales (SiO2+Al2O3+Fe2O3+H2O) Process Flow Char
Manufacturing of Portland Cement
Manufacturing Process (Dry – Semi Dry - Wet) 1. Crushing and Proportioning Limestone rock is the principal raw material, the first step after quarrying in the processes is the primary crushing. Mountains of rock are fed through crushers capable of handling pieces as large as an oil drum. The first crushing reduces the rock to a maximum size of about 15 cm (6 po). The rock then goes to secondary crushers or hammer mills for reduction to about 7.5 cm or smaller.
Manufacturing Process (Dry – Semi Dry - Wet) 2. Raw milling & Blending The next step in the process is to grind the above particles to a size of 90 microns or less which is done in a raw mill, a closed circuit ball mill equipped with high efficiency separator. After achieving the 90 microns size the fine grinded material also known as raw meal is sent to the continuous blending silos (CFC) for homogenization & extracted by means of load cell hopper for the next step which is feeding to the kiln pre heaters.
Manufacturing Process (Dry – Semi Dry - Wet) 3. Pyro processing The raw material is heated to exceeding 1,450 °C (2,700 degrees F) in huge cylindrical steel rotary kilns lined with special firebrick. Kilns are frequently as much as 3.7 M (12 pi) in diameter, large enough to accommodate an automobile and longer in many instances than the height of a 40-story building. Kilns are mounted with the axis inclined slightly from the horizontal(50o). The finely ground raw material or the slurry is fed into the higher end. At the lower end is a roaring blast of flame, produced by precisely controlled burning of powdered coal, oil or gas under forced draft.
Manufacturing Process (Dry – Semi Dry - Wet) 4. Burning and cooling As the material moves through the kiln, certain elements are driven off in the form of gases. The remaining elements unite to form a new substance with new physical and chemical characteristics. The new substance, called clinker, is formed in pieces about the size of marbles. Clinker is discharged red-hot from the lower end of the kiln and generally is brought down to handling temperature in various types of coolers. The heated air from the coolers is returned to the kilns, a process that saves fuel and increases burning efficiency.
Manufacturing Process (Dry – Semi Dry - Wet)
5. Cement milling, Storage & Packing Portland cement, the basic ingredient of concrete, is a closely controlled chemical combination of calcium, silicon, aluminum, iron and small amounts of other ingredients to which gypsum is added in the final grinding process to regulate the setting time of the concrete. Lime and silica make up about 85% of the mass. Common among the materials used in its manufacture are limestone, shells, and chalk or marl combined with shale, clay, slate or blast furnace slag, silica sand, and iron ore. The above mixture
Manufacturing Process (Dry – Semi Dry - Wet)
Cement Chemistry In cement chemistry, the individual oxides and clincker compounds are expressed by their abbreviations Short Hand Notation C (CaO, calcium oxide) A (Al2O3, alumina) S (SiO2, silica) S (SO3, sulfate) H (H20, water) Reactive Compounds C3S (tricalcium silicate) C2S (dicalcium silicate) C3A (tricalcium aluminate) CSH2 (gypsm) C4AF (tetra-calcium alumino ferrite)
Cement Chemistry Compounds of Portland Cement
Other Compounds Magnesium Oxide, MgO Calcium Oxide, Lime, CaO Alkali, Na2O, K2O equivalent Na2O=(Na2O+0.46 K2O) limited to about 1-2%